1 Public Report Document ID Author Matts Björck Reviewed by Version 1.0 Lisette Åkerman (QA) Approved by Jan Sarnet Status Approved Reg no Date Reviewed date Approved date Page 1 (13) Estimation of oxide growth on joint Abstract A previously developed model of the oxidation kinetics of pure copper in an Ar/O 2 atmosphere is applied to the case of Friction Stir Welding of copper canisters. In order to apply the model the experimental temperature history of the joint surfaces together with metallographic is used as input. Ambient oxygen levels results in maximum oxygen content of about 100 wt-ppm in the weld material. If the oxygen concentration in the surrounding atmosphere during welding is lowered to 100 mol-ppm the resulting increase in the oxygen concentration in the weld material will be below 1 wt-ppm. At these and lower oxygen concentrations the native oxide film formed prior to welding is a significant contribution to the increase in the oxygen content in the weld material. PO Box 925, SE Oskarshamn Visiting address Gröndalsgatan 15 Phone Fax Seat Stockholm
2 Public 1.0 Approved 2 (13) 1 Introduction As friction stir welding (FSW) is a solid state joining process most produced welds contains elevated amounts of oxygen. This is caused by a combination of elevated temperatures and access to oxygen prior to the joining of the joint surfaces. The streaks of embedded oxide particles for the copper welds produced by SKB have not been shown to have a detrimental effect on the mechanical properties (Andersson-Östling and Sandström 2009) nor have they shown an effect in previous corrosion experiments (Gubner and Andersson 2007). However, the oxide streaks are considered an imperfection and should, consequently, be minimized. One way to reduce the amount of oxides is to lower the oxygen content in the atmosphere around the joint line. This is usually done by protecting the joint surfaces with an inert gas, such as argon. The FSW machine at the canister laboratory has been fitted with a gas shield during the last years. When developing such a gas shield it is natural to consider which oxygen partial pressure should be kept within the shield. In order to answer this question an experimental program has been set up at the canister laboratory. The first step consisted of a literature study combined with an experimental study (SKBdoc ) to determine the oxidation kinetics of copper surfaces exposed to various oxygen partial pressures. This resulted in a model that can calculate the amount of oxide formed given the temperature, time and oxygen content available. The remaining part, which will be dealt with in this report, consists of using the temperature history at the joint line to estimate the amount of oxide formed during welding for different oxygen partial pressures. 2 Theory 2.1 Oxidation kinetics The oxidation kinetics of copper was reviewed and completed with experimental measurements in Oxidation kinetics of copper at reduced oxygen partial pressures (SKBdoc ). As the oxygen partial pressure is decreased there will be a transition from parabolic to linear kinetics. The parabolic rate constant has a limited dependence on the oxygen pressure whereas the linear rate constant has a linear dependence on the oxygen partial pressure. The rate equation can be written as + =, (2-1) Where t is the time and x the weight per area unit of oxide formed. and are the parabolic and linear rate constants, respectively. This equation can be re-cast into a differential form which is applicable when and are time dependent, for example when the oxygen partial pressure or the temperature are changing. The differential form is consequently written as + =. (2-2) The differential equation can be integrated numerically as shown in the implementation in Appendix A. The constants and can be parameterized by using an Arrhenius expression for the temperature dependent part and a power law for the oxygen partial pressure, which becomes, =,,, +,, (2-3) and, =,. (2-4) The parameters in the above equations are given in Table 2-1. These parameters are the results of fitting the model parameters to thermogravimetric data in a range from 100 mol-ppm to
3 Public 1.0 Approved 3 (13) 21 mol-%. For further details the reader is referred to Oxidation kinetics of copper at reduced oxygen partial pressures (SKBdoc ). Table 2-1. The parameters used to describe the oxidation kinetics. Parameter Value /( ) 27 / 1.04,, 21 % , 634 /( ), 248 /, /( ), 103 / Model of oxidation during FSW Figure 2-1. A cartoon of the concept used to model the FSW process viewed along the rotation axis of the probe. The FSW model used for calculating the amount of oxidation is shown in Figure 2-1. The probe will rotate and pull a certain amount of material with it, the shear layer. The layer will have an extension of from the probe. As the joint surface move into the shear layer it will be heavily deformed and bonded, see Sealing of the canister SKBdoc for more details. When the joint surfaces fuses together it is assumed that the oxygen will not be able to further oxidize the material. Also, the oxidation is assumed to follow the model described above. This thought model contains a number of simplifications. Firstly, the current oxidation model as presented was developed for surfaces freely exposed to the environment. The joint surfaces will be clamped under a significant pressure. This could reduce the access of the oxygen to the joint surfaces. Secondly, the material flow around the probe will break up the oxide films and disperse it as can be seen in Sealing of the canister SKBdoc In addition, the material flow is not two dimensional (Källgren 2010). The calculations are therefore expected to overestimate the amount of oxidation. This overestimation will not apply close to the outer surface of the weld where the shoulder, see Figure 2-2, can mix in oxides from the outer surface into the weld. It should be noted that this outer part of the weld (5 mm) is machined away.
4 Public 1.0 Approved 4 (13) Figure 2-2. A side view of the probe and shoulder relative to the outer surface of the weld. 2.3 Effect of surface oxides on total oxygen content The tube and lid material used in trial production is oxygen free phosphorus copper (Cu- OFP) which is specified to have an oxygen content less than 5 wt-ppm (SKB 2010). Typical sample sizes for measuring the oxygen content by melt extraction are a cube with side = 5 mm. It is instructive to estimate the effect of oxidized joint surfaces on the measured oxygen content. Assuming that the oxidized surfaces will largely remain intact during the process, which is a pessimistic assumption given the stirring action of the FSW tool, the calculations simplifies to calculating the oxygen content in the aforementioned cube containing an oxide layer of thickness. The molar density of a component can be written as =, where is the mass density, is the molar mass and is the volume. The volume of the oxide layer is = and the total volume of the sample is =. When copper oxidize two different copper oxides can form, either cupric oxide or cuprous oxide which has different oxygen molar densities, see Table 2-2. According to Zhu et al. (2006) dominates the oxide layer formed in air for temperatures above 350. This is also the assumption used in SKBdoc to transform the measured and modelled weight gains to thicknesses. Consequently, the same assumption will be used here to transform the modelled thicknesses to weight values as this will remove any systematic errors. The base material has an oxygen concentration,, =,. The concentration of oxygen in the sample is =, +, where it has been assumed that. The constant +, = +,, =. Table 2-2. Material properties used in the calculation of the oxygen content. Compound Molar mass, [ / ] Density, [ / ] [ / ] The oxygen content in the sample as a function of the oxide thickness as given by the expression above can be seen in Figure 2-3. In order for the increase in oxygen content in the sample to be on the
5 Public 1.0 Approved 5 (13) same order of magnitude as the base material (< 5wt-ppm) the oxide layer thickness has to be about 0.1. Figure 2-3. The increase in oxygen content as a function of oxide thickness on a micro meter scale (left) and on a nano meter scale (right). As a comparison the base material Cu-OFP has oxygen content of below as indicated by the blue dotted line. 3 Experimental details The temperature measurement during welding were conducted by placing type K thermocouples close to the joint line by drilling holes into the ring and lid to be welded. A total of 18 thermocouples were placed around the weld to monitor the temperature at several points. Three of the thermocouples were placed to create a depth profile 2 mm from the joint line. The temperatures were sampled at 8 Hz with a Eurotherm 6100 A data logger. A more detailed description of the experimental setup can be found in Oxidation kinetics of copper at reduced oxygen partial pressures (SKBdoc ). The metallographic examinations were taken from sectioning exit holes from weld FSW99. The samples were metallographically prepared and studied with a stereomicroscope macroscopically as well as with a microscope to reveal the details of remaining joint. The results are presented in Metallographic examination of exit holes in FSWL99 (SKBdoc ). 4 Results and Discussion 4.1 Metallographic investigation An example of a prepared sample is shown in Figure 4-1. The distance between the rim of the hole to the non-bonded joint is = 2.5. This distance will decrease to = 1.6 at the tip of the tool and further increase to = 2.8 about 1.5 from the surface of the canister.
6 Public 1.0 Approved 6 (13) Figure 4-1. Two macrographs(id: FSW deg T2 and FSW deg T3 ) an exit hole. The bright yellow horizontal line to the right is the unbonded remaining joint line. The right section is taken closer to the root of the weld whereas the left is taken closer to the surface. The more fine grained area is the welded material. The semicirculair features seen on the left picture are optical artefacts from the microscope. See SKBdoc for further details. 4.2 Temperature profile During the measurements the probe broke before arriving to the final three thermocouples that were placed at the joint line. Therefore only one thermocouple, the one closest to the surface, gives a, for the process, valid reading. The temperature evolution for that thermocouple is shown in Figure 4-2. The first maxima arise due to the heating during the start sequence; the thermocouples are located directly below the plunge position. After welding around the canister the probe arrives to the thermocouple position again to complete the joint. This creates the leftmost and highest peaks in the graph. Using the speed of the machine and the peaks in the thermocouples located at the depth from the surface at a distance of 180 away from the outermost thermocouple it is possible to estimate where the centre of the tool crosses the thermocouple position (calculated to occur at time 14:11:45). Then using the thickness of the shear layer measured in section 4.1 combined with the measured diameter of the exit hole ( ) an interval where the joint was created can be estimated. These distances can be recalculated to time by using the welding speed, 80 /. The resulting points are shown in Figure 4-3. As the thermocouple is placed closer to the surface it can be expected that the maximum temperature reached is about 800. If the position of the joining at the root is used instead the maximum temperature would be 900 that would be constant for 5 assuming that the temperature profile would be constant. However, the thermocouple is located at the outer surface and consequently the temperature used in the following calculations will assume that the surfaces join just before the first drop in the temperature readings.
7 Public 1.0 Approved 7 (13) Figure 4-2. Three thermocouples recordings for the thermocouples located closest to the joint line. distance from the outer surface of the weld. denote the Figure 4-3. The temperature as a function of time for the thermocouple located closest to surface, red line, with vertical lines showing the different events that are discussed in the text. The temperature recorded under the starting position will probably not be the one that cause the most oxidation. Instead the position that will have the highest temperature for the longest time will be the joint surfaces next to the beginning of the joint line sequence as shown in Figure 4-4. As no measurements were made at this position the temperatures will be estimated instead. The highest measured temperature in weld FSWL94 (SKBdoc ) that was not part of the weld zone was the thermocouple located at with a maximum temperature of 713. Consequently this data set has been used to replace the beginning of the data set in Figure 4-2 for = 5. This will be used as one of two cases analysed further in the next section.
8 Public 1.0 Approved 8 (13) Figure 4-4. A picture denoting the different sequences during welding: The dwell and start sequence (1), the downward sequence(2), the joint line sequence (3), the overlap sequence (4) and the parking sequence (5). 4.3 Oxidation evolution Using the temperature curves discussed above as input in the oxidation kinetics model the evolution of the oxide thickness as a function of time for different scenarios can be calculated. Glow Discharge Optical Emission depth profiling (SKBdoc ) has shown that using the joint preparation procedure currently used 1 before welding the oxide thickness is below 10. However, other labs have reported that clean copper surfaces have an oxide thickness of about 1, see references in Oxidation kinetics of copper at reduced oxygen partial pressures (SKBdoc ). Therefore both of these scenarios will be used in the subsequent calculations. Two different temperature evolutions will be used. One of them is representing an estimation of the beginning of the joint line sequence and the other a measured curve below the starting hole Atmospheric conditions The resulting oxidation growth curve for atmospheric conditions, 21mol-%, is shown in Figure 4-5. As can be seen in the figure the oxide thickness reaches a thickness of 4 for the temperature evolution corresponding to the beginning of the joint line sequence. In Oxidation kinetics of copper at reduced oxygen partial pressures (SKBdoc ) some spallation was observed during the experiments. This can occur upon rapid temperature changes and thick films. This can be modelled as a restart of the oxidation after a sharp temperature drop. Doing this calculation (not shown here) yield a maximum oxide thickness of 5 for the temperature evolution at the beginning of the joint line sequence. Consequently, the effect of spallation is estimated to be 20 % in this case. 1 The preparations are dry milling of joint surfaces, abrasive cleaning and spraying with ethanol and subsequent wiping using lint free paper.
9 Public 1.0 Approved 9 (13) Figure 4-5. The oxide thickness (top) as a function of time for mol-% and temperature according to the lower panel. Full lines correspond to a position under the starting hole and dashed line to the beginning of the joint line sequence Reduced oxygen content If the oxygen partial pressure is reduced into the range of linear kinetics the growth rate will decline proportional to the oxygen pressure. At 100 mol-ppm, see Figure 4-6, the oxide thickness will be reduced two orders of magnitude as compared to atmospheric conditions. At these oxygen concentrations also the initial oxide thickness plays a significant role. Reducing the oxygen concentration further to 50 mol-ppm lowers the oxide thickness further as can be seen in Figure 4-7. The lowest oxygen concentration used when developing the model was 100 mol-ppm. However, if another physical mechanism would be in control at lower oxygen concentrations it should lower the growth rate further in order to be the rate controlling step. Figure 4-6.The oxide thickness (top) with initial thickness of (black) and (red) at mol-ppm as a function of time. The lower panel shows the temperature evolution used as input in the simulations. Full lines correspond to a position under the start hole and dashed lines to the beginning of the joint line sequence.
10 Public 1.0 Approved 10 (13) Figure 4-7. Same information as in Figure 4-6 for mol-ppm. 4.4 Effects on the oxygen levels in the weld At atmospheric conditions the oxygen layer thickness on one surface is calculated to be 4, thus the total oxide thickness would be 8 for two surfaces. According to Figure 2-3 this translates to an oxygen content of 100 wt-ppm in a sample. This is higher than the maximum value seen in FSW27 (SKBdoc ), 44 ± 12 wt-ppm, that was produced in air. That can be expected as the probe disperses the oxide layer in the weld zone and thus lower the oxygen content compared to the simplified model. If oxygen concentration in the environment is reduced to 100 mol-ppm the maximum oxide thickness will be which translate to an increase in oxygen content of wt-ppm. Reducing the oxygen concentration further to 50 mol-ppm causes the increase in oxygen concentration in the sample to be < 0.5 wt-ppm. 5 Conclusions Given that the oxide layer on the joint surfaces are below 10 and that the oxygen concentration at the weld surfaces are below 100 mol-ppm the calculations presented here indicate that the increase in oxygen content in the weld zone will be below 1 wt-ppm. An oxygen concentration of 100 mol-ppm will keep the oxide film at the same order of magnitude as for an initial oxide thickness of 10. An oxygen partial pressure of 50 mol-ppm and an initial oxide thickness of 1 will keep the oxide thickness formed below 10 nm. 6 References Andersson-Östling H C M, Sandström R, Survey of creep properties of copper intended for nuclear waste disposal. SKB TR-09-32,. Gubner R, Andersson U, Corrosion resistance of copper canister weld material. SKB TR-07-07,. Källgren T, Investigation and modelling of friction stir welded copper canisters. PhD thesis. Royal Institute of Technology, Sweden.
11 Public 1.0 Approved 11 (13) SKB, Design, production and initial state of the canister. SKB TR-10-14, Svensk Kärnbränslehantering AB. Zhu Y, Mimura K, Lim J-W, Isshiki M, Jiang Q, Brief review of oxidation kinetics of copper at 350 C to 1050 C. Metallurgical and Materials Transactions A 37, Unpublished documents SKBdoc id, version Title Publisher, year ver 1.0 Technical report of SKB FSW chemical analysis Luvata Pori Oy, ver 1.0 FSWL94 Measurement of temperatures and surrounding oxygen levels during welding SKB, ver. 1.0 Metallographic examination of exit holes in FSWL99 SKB, ver 1.0 Undersökning av rengöringsmetoder och oxidation av kopparytor i ädelgas med GD-OES. (In Swedish.) ver 1.0 Oxidation kinetics of copper at reduced oxygen partial pressures SKB, 2013 SKB, ver 1.0 Sealing of the canister SKB, , ver 1.0 Technical report of SKB FSW chemical analysis rev2, Luvata Luvata Pori Oy, 2010
12 Public 1.0 Approved 12 (13) 7 Appendix A The program code, written in Python, used for the simulations is given below. # -*- coding: utf-8 -*- """ A script to estimate the growth of Cu2O at different conditions. Programmer: Matts Bjorck, Last modified: """ from numpy import * # Constants used pc, ppm = 1e-2, 1e-6 h, min, s = 3600., 60., 1. _plot = True # Settings for the calculations out_file = "O50ppm_d010nm" # Initial oxide thickness d0 = #mum # Set the oxygen partial pressure used in the calculations oxygen_cont = 50*ppm def x_to_d(x): """Transforms the weight gain, x, in g/cm2 to thickness, d, in mum""" return x*1.46e4 def d_to_x(aa): """Transforms the thickness, d, in mum to weight gain,x, in g/cm2""" return AA/1.46e4 def calc_weight(time, temp, p_oxygen, x0): """Calculates the weight given the parameters with combination of linear and parabolic rate constantas according to Ronnqvist and Fischmeister. """ # Previously fitted constants A_p1 = 634 #g2/cm4/s A_p2 = 8.67e-4 #g2/cm4/s E_p1 = 248e3 #J/mol E_p2 = 103e3 #J/mol A_l = 1.19e-7 #g/cm2/s E_l = 27e3 #J/mol n_l = 1.04 n_p = 0.0 F_p = 0.83 p_refp = 0.21 p_refl = 1000e-6 # Transforming deg C to deg K T = temp # Defing constants # R - the gas cosntant R = #J/mol/K kp = F_p*(p_oxygen/p_refp)**n_p*(A_p1*exp(-E_p1/R/T) + A_p2*exp(-E_p2/R/T)) kl = (p_oxygen/p_refl)**n_l*a_l*exp(-e_l/r*(1./t - 1./ )) # Setting the first element to the pre-oxidezed value x = [x0] #Doing a forward integration for each time step for i in range(1,len(time)): dt = time[i] - time [i-1] av_kl = (kl[i] + kl[i-1])/2. av_kp = (kp[i] + kp[i-1])/2. dx = dt/(1.0/av_kl + 2*x[-1]/av_kp) x.append(x[-1] + dx) #return 0.5*(-kp/kl + sqrt((kp/kl)**2 + 4*kp*(time))) return array(x) # Load temperatures for the position under the start pos. A = loadtxt('data_for_oxidationslast.txt', delimiter = None, skiprows = 2) print A.shape temp_start = A[:,1] time_start = A[:,0]-A[6000,0]
13 Public 1.0 Approved 13 (13) def create_worst_tempcase(): '''Assembles data for a worst case when the probe reach the joint line''' A1 = loadtxt('data_for_oxidationslast.txt', delimiter = None, skiprows = 2) A2 = loadtxt('tempdata_1815deg.txt', delimiter = None, skiprows = 2) offset1 = (-0/ )/0.125 offset2 = ( / )/0.125 # Slice out the relevant parts maxind = min(a1.shape-offset1, A2.shape-offset2) cross = argmin(abs(a1[offset1:offset1 + maxind,1]-a2[offset2:offset2 + maxind,1])) merged = r_[a2[offset2:offset2+cross,1], A1[offset1 + cross:,1]] time = arange(len(merged))*0.125 return time, merged # Load the data corresponding to the "worst case" time_worst, temp_worst = create_worst_tempcase() # Tranform the initial oxide thickness to weight x0 = d_to_x(d0) # Calculate the "worst" case d_worst = x_to_d(calc_weight(time_worst, temp_worst, oxygen_cont, x0)) # Calculate the thickness under the start hole d_start = x_to_d(calc_weight(time_start, temp_start, oxygen_cont, x0)) # saving the results to file f = open(out_file + '_worst.dat','w') f.write('time [s]\t Temperature [deg C]\t Oxygen content\t Oxide thickness [mum]\n') savetxt(f, c_[time_worst, temp_worst, oxygen_cont*(time_worst*0 + 1), d_worst]) f.close() f = open(out_file + '_start.dat','w') f.write('time [s]\t Temperature [deg C]\t Oxygen content\t Oxide thickness [mum]\n') savetxt(f, c_[time_start, temp_start, oxygen_cont*(time_start*0 + 1), d_start]) f.close() # Optional plotting if _plot: from pylab import * subplot(211) plot(time_worst[:]/60, d_worst) plot(time_start[:]/60, d_start) ylabel('thickness [mum]') subplot(212) plot(time_worst/60., temp_worst) plot(time_start/60., temp_start) ylabel('temperature [deg C]') show()
PDF rendering: DokumentID 1473479, Version 1., Status Godkänt, Sekretessklass Öppen Analyses on copper samples from Micans P. Berastegui, M. Hahlin, M. Ottosson, M. Korvela, Y. Andersson, R. Berger and
Chemistry Lab Report Aim: The combustion of organic compounds produces large quantities of energy. These compounds range from that of alkanes, to alkenes to even alcohols. Ethanol is a commonly used fuel
Technical Report TR-1-29 Damage tolerance analysis of canister inserts for spent nuclear fuel in the case of an earthquake induced rock shear load Peter Dillström, Tobias Bolinder Inspecta Technology AB
MATEC Web of Conferences43, 03005 ( 016) DOI: 10.1051/ matecconf/ 016 4303005 C Owned by the authors, published by EDP Sciences, 016 Process Parameters Optimization for Friction Stir Welding of Pure Aluminium
Molecular Mass by Freezing Point Depression Kyle Miller November 28, 2006 1 Purpose The purpose of this experiment is to determine the molecular mass of organic compounds which are dissolved in a solvent
THE SOLUBILITY OF A SALT IN WATER AT VARIOUS TEMPERATURES 2007, 1995, 1991 by David A. Katz. All rights reserved. Permission for academic use provided the original copyright is included. OBJECTIVE To measure
RECALL FIRST CLASS: Q K Head Difference Area Distance between Heads Q 0.01 cm 0.19 m 6cm 0.75cm 1 liter 86400sec 1.17 liter ~ 1 liter sec 0.63 m 1000cm 3 day day day constant head 0.4 m 0.1 m FINE SAND
Production of ductile iron castings without feeders Possibilities of producing ductile iron castings in green sand mould without feeders by means of "ingate" feeding and control of the graphite precipitation
Copper corrosion processes in the Cu-O-H system, and their role in long-term safety assessments Christina Lilja 2009-11-16 Outline Scientific knowledge base thermodynamics the use of experimental results
Electronic Materials Devices and Fabrication Layering: Thermal Oxidation Dr. S. Parasuraman Department of Metallurgical and Materials Engineering Indian Institute of Technology, Madras Module - 01 Lecture
Boltzmann Distribution Law The motion of molecules is extremely chaotic Any individual molecule is colliding with others at an enormous rate Typically at a rate of a billion times per second We introduce
Product Information Mylar polyester film Physical-Thermal Properties Mylar polyester film retains good physical properties over a wide temperature range ( 7 to 15 C [ 9 to 3 F]), and it is also used at
Heats of Transition, Heats of Reaction, Specific Heats, and Hess s Law GOAL AND OVERVIEW A simple calorimeter will be made and calibrated. It will be used to determine the heat of fusion of ice, the specific
C O N T R A C T W O R K R E P O R T C O N F I D E N T I A L Exposure of Copper in Äspö Groundwaters Author: Claes Taxén Department: 70 Phone: 08-6741739 E-mail: firstname.lastname@example.org Date: 2009-04-16 Your
Surface Engineering Solutions Rebuild, Repair and Protect Industrial Equipment Whatever You Rebuild, Repair and Protect...... Find the Right Solution! Henkel's Solutions for all Surface Engineering Needs
Naue GmbH&Co.KG Quality Control and Quality Assurance Manual For Geomembranes July 2004 V.O TABLE OF CONTENTS 1. Introduction 2. Quality Assurance and Control 2.1 General 2.2 Quality management acc. to
Laboratory exercise No. 4 Water vapor and liquid moisture transport Water vapor transport in porous materials Due to the thermal conductivity of water and other unfavourable properties and effects in porous
th International Conference on Structural Mechanics in Reactor Technology (SMiRT ) Espoo, Finland, August 9-4, 9 SMiRT -Division 3, Paper 56 Investigations of a Long-Distance MW Heat Transport System with
Heat Transfer Prof. Dr. Aloke Kumar Ghosal Department of Chemical Engineering Indian Institute of Technology, Guwahati Module No. # 02 One Dimensional Steady State Heat Transfer Lecture No. # 05 Extended
Chemistry 212 VAPOR PRESSURE OF WATER LEARNING OBJECTIVES The learning objectives of this experiment are to explore the relationship between the temperature and vapor pressure of water. determine the molar
THE WAY TO SOMEWHERE Sub-topics 1 Diffusion Diffusion processes in industry RATE PROCESSES IN SOLIDS At any temperature different from absolute zero all atoms, irrespective of their state of aggregation
1 of 9 Supporting document to NORSOK Standard C-004, Edition 2, May 2013, Section 5.4 Hot air flow A method utilizing Computational Fluid Dynamics (CFD) codes for determination of acceptable risk level
E 490 Fundamentals of Engineering Review Fluid Mechanics By M. A. Boles, PhD Department of Mechanical & Aerospace Engineering North Carolina State University Archimedes Principle and Buoyancy 1. A block
A METALLOGRAPHIC INVESTIGATION OF ANCIENT COOKING UTENSILS D. Kountouras, S. Papanikolaou, P. Serdaris, S. Maropoulos Mechanical Engineering Department, Technical Educational Institute of Western Macedonia,
Determination of the enthalpy of TEC Related concepts First law of thermodynamics, Hess s law of constant heat summation, enthalpy of combustion, enthalpy of formation, heat capacity. Principle The bomb
Experiment 2 Colligative Properties of Solutions Introduction: Consider a hypothetical cooling curve which describes the changes in phase of a pure substance in which heat is lost at a steady rate at constant
A cart full of water travels horizontally on a frictionless track with initial velocity v. As shown in the diagram, in the back wall of the cart there is a small opening near the bottom of the wall that
Chapter 13 - LIQUIDS AND SOLIDS Problems to try at end of chapter: Answers in Appendix I: 1,3,5,7b,9b,15,17,23,25,29,31,33,45,49,51,53,61 13.1 Properties of Liquids 1. Liquids take the shape of their container,
AP Physics 1 and 2 Lab Investigations Student Guide to Data Analysis New York, NY. College Board, Advanced Placement, Advanced Placement Program, AP, AP Central, and the acorn logo are registered trademarks
Physical Properties of a Pure Substance, Water The chemical and physical properties of a substance characterize it as a unique substance, and the determination of these properties can often allow one to
Physics Equipotential Lines and Electric Fields Plotting the Electric Field MATERIALS AND RESOURCES ABOUT THIS LESSON EACH GROUP 5 alligator clip leads 2 batteries, 9 V 2 binder clips, large computer LabQuest
Smart Magnets for Precision Alignment Smart Magnets for Precision Alignment in Product Design Correlated Magnetics Research creates specially engineered smart magnets for use in product design that are
Catalog No. AP6356 Publication No. 6356A Molar Mass by Freezing Point Depression AP Chemistry Laboratory #4 Introduction A procedure for determining the molar mass of a substance is very useful to chemists.
HWR 431 / 531 HYDROGEOLOGY LAB SECTION LABORATORY 2 DARCY S LAW Introduction In 1856, Henry Darcy, a French hydraulic engineer, published a report in which he described a series of experiments he had performed
Pin & Vee Block Test Machine Picture of the apparatus Used in Standard Test Methods ASTM Standards D 2670, D2626, D3233, D5620 Federal Test Methods FTM-791-3807.1, FTM-791-3812.1 Chrysler Corporation 461-C-84-01,
T A B L E T 1 1 of 7 Tests & Inspection Cable PCUT & PCUT-A (Table T1) T E S T S A N D I N S P E C T I O N C A B L E P C U T A N D P C U T - A No. Test Scale MOC Requirements G 20:10:001:01 Defined Test
Basic Concepts of Thermodynamics Every science has its own unique vocabulary associated with it. recise definition of basic concepts forms a sound foundation for development of a science and prevents possible
The Kinetic Theory of Gases Sections Covered in the Text: Chapter 18 In Note 15 we reviewed macroscopic properties of matter, in particular, temperature and pressure. Here we see how the temperature and
Carbon Dioxide and an Argon + Nitrogen Mixture Measurement of C p /C v for Argon, Nitrogen, Stephen Lucas 05/11/10 Measurement of C p /C v for Argon, Nitrogen, Carbon Dioxide and an Argon + Nitrogen Mixture
Experiment 1: Colligative Properties Determination of the Molar Mass of a Compound by Freezing Point Depression. Objective: The objective of this experiment is to determine the molar mass of an unknown
INTERNATIONAL BACCALAUREATE BACCALAURÉAT INTERNATIONAL BACHILLERATO INTERNACIONAL M01/430/H(3) PHYSICS HIGHER LEVEL PAPER 3 Wednesday 16 May 2001 (morning) Name Number 1 hour 15 minutes INSTRUCTIONS TO
Fluids and Solids: Fundamentals We normally recognize three states of matter: solid; liquid and gas. However, liquid and gas are both fluids: in contrast to solids they lack the ability to resist deformation.
Lecture 5 Physics of Welding Arc I This chapter presents fundamentals of welding arc, mechanisms of electron emission, different zones in welding arc, electrical aspects related with welding arc and their
Liquid Fuel Burning Behavior in Ice Cylinders A Major Qualifying Project Report Submitted to the Faculty of the WORCESTER POLYTECHNIC INSTITUTE In partial fulfillment of the requirements for the Degree
Chapter 4 and 5 solutions 4.4. Three different washing solutions are being compared to study their effectiveness in retarding bacteria growth in five gallon milk containers. The analysis is done in a laboratory,
International Progress Report IPR-02-64 Äspö Hard Rock Laboratory Temperature Buffer Test Report for retaining plug and anchoring Richard Bäck Äspö HRL September 2002 Svensk Kärnbränslehantering AB Swedish
Supporting Information Wiley-VCH 2007 69451 Weinheim, Germany Methanol Behavior in Direct Methanol Fuel Cells Younkee Paik, Seong-Soo Kim, and Oc Hee Han * Experimental Section Preparation of MEA: Standard
Lecture 3: Electron statistics in a solid Contents Density of states. DOS in a 3D uniform solid.................... 3.2 DOS for a 2D solid........................ 4.3 DOS for a D solid........................
Experiment #5: Qualitative Absorption Spectroscopy One of the most important areas in the field of analytical chemistry is that of spectroscopy. In general terms, spectroscopy deals with the interactions
1. Which of the following statements about a spring-block oscillator in simple harmonic motion about its equilibrium point is false? (A) The displacement is directly related to the acceleration. (B) The
Integration of a fin experiment into the undergraduate heat transfer laboratory H. I. Abu-Mulaweh Mechanical Engineering Department, Purdue University at Fort Wayne, Fort Wayne, IN 46805, USA E-mail: email@example.com
Friction Stir Welding of Stainless Steel and Nickel Base Alloys R.J. Steel, T.W. Nelson, C.D. Sorensen, Y.S. Sato, C.J. Sterling, and S.M. Packer Acknowledgements Material provided by: Haynes International
Chemistry 2007 Sample assessment instrument and indicative responses Extended experimental investigation This sample is intended to inform the design of assessment instruments in the senior phase of learning.
5. DIMENSIONS, TOLERANCES AND SURFACE 5.1 Dimension, Tolerances and Related Attributes 5.2 Surfaces 5.3 Effect of Manufacturing Processes Introduction Dimensions the sizes and geometric features of a component
CHAPTER 9 MOLAR MASS OF A GAS THE MOLAR MASS OF ALMOST ANY GAS can be accurately determined within a single laboratory period using 60 ml plastic syringes. The mass of a plastic syringe is determined with
CHANGE OF AIR TEMPERATURE WITH ALTITUDE, ATMOSPHERIC STABILITY AND AIR POLLUTION Vertical motion of air governs many atmospheric processes, such as the formation of clouds and precipitation and the dispersal
Rock Bolt Condition Monitoring Using Ultrasonic Guided Waves Bennie Buys Department of Mechanical and Aeronautical Engineering University of Pretoria Introduction Rock Bolts and their associated problems
The first scheduled quiz will be given next Tuesday during Lecture. It will last 5 minutes. Bring pencil, calculator, and your book. The coverage will be pp 364-44, i.e. Sections 0.0 through.4. 0.7 Theory
Safety precautions Naphthalene is harmful if swallowed. May cause cancer. Is further very toxic to aquatic organisms and can have long-term harmful effects in bodies of water. Equipment 1 Bomb calorimeter
Laboratory 8 Fatigue Testing Objectives Students are required to understand principle of fatigue testing as well as practice how to operate the fatigue testing machine in a reverse loading manner. Students
KWANG SING ENGINEERING PTE LTD 1. INTRODUCTION This report represents the soil investigation works at Aljunied Road / Geylang East Central. The objective of the soil investigation is to obtain soil parameters
Fluid Mechanics Prof. T. I. Eldho Department of Civil Engineering Indian Institute of Technology, Bombay Lecture No. # 36 Pipe Flow Systems Welcome back to the video course on Fluid Mechanics. In today
P2800 Fall 2008 Questions (Total - 20 points): 1. Of the noble gases Ne, Ar, Kr and Xe, which should be the most chemically reactive and why? (0.5 point) Xenon should be most reactive since its outermost
.1.1 Measure the motion of objects to understand.1.1 Develop graphical, the relationships among distance, velocity and mathematical, and pictorial acceleration. Develop deeper understanding through representations
Head Loss in Pipe Flow ME 123: Mechanical Engineering Laboratory II: Fluids Dr. J. M. Meyers Dr. D. G. Fletcher Dr. Y. Dubief 1. Introduction Last lab you investigated flow loss in a pipe due to the roughness
Assessment Chapter Test B Chapter: Measurements and Calculations PART I In the space provided, write the letter of the term or phrase that best completes each statement or best answers each question. 1.
KINETIC THEORY AND THERMODYNAMICS 1. Basic ideas Kinetic theory based on experiments, which proved that a) matter contains particles and quite a lot of space between them b) these particles always move
SKBdoc id 1415873 Supplementary material in addition to SR-Site modeling report TR-10-11 as requested by SSM 3.1. Analysis of saturation intervals concerning long time safety during the hydration process
User Manual Keofitt Simplex Sampling valve s o m e p e o p l e w o u l d n t g a m B l e w i t h t h e i r s a m p l e t m Introduction: Manufacturer: Keofitt A/S, Industrivænget 6-8 5700 Svendborg Denmark
Corrosion Test of US Steels in Lead-Bismuth Eutectic (LBE) and Kinetic Modeling of Corrosion in LBE Systems N. Li, X. He MSK764, Los Alamos National Laboratory, Los Alamos, NM 87545, U.S.A. firstname.lastname@example.org
MACHINE RECCOMENDATIONS PVC requires reciprocating screw injection moulding machine with a plasticising screw to produce homogeneous melt. It is recommended that a shot weight of the part should take two
Laboratory 14 Vapor Pressure and the Heat of Vaporization Objectives Use experimental techniques to record temperature and volume data for known and unknown compounds in which the liquid and gas are in
The Physical Sciences Initiative Chemistry Inservice D A T A L O G G I N G Heat of Reaction for Graphic Calculator & Computer Nov 2001 1 Heat of Reaction. A Styrofoam cup calorimeter is used in this experiment
TELEDYNE HASTINGS TECHNICAL PAPERS INSTRUMENTS A LAMINAR FLOW ELEMENT WITH A LINEAR PRESSURE DROP VERSUS VOLUMETRIC FLOW Proceedings of FEDSM 98: June -5, 998, Washington, DC FEDSM98 49 ABSTRACT The pressure
Introduction to Metallography Metallography has been described as both a science and an art. Traditionally, metallography has been the study of the microscopic structure of metals and alloys using optical
RESEARCH PAPERS FACULTY OF MATERIALS SCIENCE AND TECHNOLOGY IN TRNAVA SLOVAK UNIVERSITY OF TECHNOLOGY IN BRATISLAVA 2014 Volume 22, Special Number DIESEL EFFECT PROBLEM SOLVING DURING INJECTION MOULDING
AP Physics C Oscillations/SHM Review Packet 1. A 0.5 kg mass on a spring has a displacement as a function of time given by the equation x(t) = 0.8Cos(πt). Find the following: a. The time for one complete
13 Powder Metallurgical Process for the Production of Metallic Foams J. Banhart and P. Weigand Fraunhofer-Institute for Applied Materials Research, Bremen, Germany Abstract A powder metallurgical method
Excerpt from the Proceedings of the COMSOL Conference 010 Boston COMSOL Assisted Simulation of Laser Engraving Hamidreza Karbasi Conestoga College Institute of Technology and Advanced Learning School of
Concept 1: Properties of Objects and Materials Classify objects and materials by their observable properties. Kindergarten Grade 1 Grade 2 Grade 3 Grade 4 PO 1. Identify the following observable properties
Your consent to our cookies if you continue to use this website.